Abstract
Spintronics aims to utilize the spin degree of freedom for information storage and computing applications. One major issue is the generation and detection of spins via spin and charge conversion. Quantum materials have recently exhibited many unique spindependent properties, which can be used as promising material candidates for efficient spin and charge conversion. Here, we review recent findings concerning spin and charge conversion in quantum materials, including Rashba interfaces, topological insulators, twodimensional materials, superconductors, and noncollinear antiferromagnets. Important progress in using quantum materials for spin and charge conversion could pave the way for developing future spintronics devices.
Similar content being viewed by others
Introduction to pure spin current
Spintronics aims to utilize the spin degree freedom of electrons for potential applications such as novel information storage and computing.^{1,2,3} Compared to conventional devices using electron’s charge properties, spintronic devices potentially have several major advantages, including nonvolatility, faster data processing speed, higher integration densities, and less electric power consumption. The key challenges are the efficient generation and detection of pure spin current, which does not accompany any charge current, as illustrated in Fig. 1a^{1}. The pure spin current could be used as information transistors and logic devices.^{4,5,6} For example, spinbased field effect transistors can provide on and off operations via the manipulation of the spin current in the spin channel.^{4,7} As shown in Fig. 1b, the pure spin current that carries the information flows from the injector to the detector via the spin channel. Due to the spin relaxation, the spindependent chemical potential exponentially decays during the spin diffusion (Fig. 1c). Thus, for the purpose of spin transistor and logic device applications, the spin channel with long spin lifetimes and long spin diffusion length is needed. Graphene might hold the promise for this purpose since the demonstration of its fantastic spindependent properties at room temperature arising from its low spin orbit coupling and high mobility.^{8,9}
Besides serving as a transmitter of information, the spin current also carries angular momentum. As illustrated in Fig. 1a, the spin current can also be viewed as the transfer of angular momentum, which could be used for magnetization switching applications via spin–transfer torque.^{10,11} In the last several years, the spin–orbit torque, arising from pure spin current in nonmagnetic materials (NM) (Fig. 1d), can be used to switch the magnetization of adjacent ferromagnets (FM).^{12,13,14,15,16} As illustrated in Fig. 1e, the spin current provides a spin–transfer torque to the magnetization that can be expressed by
where ℏ is the reduced Plank constant, \({\hat{\mathbf m}}\) is the magnetization vector, and \({\hat{\mathbf \sigma }}\) represents the spin polarization direction of the spin current. For this purpose, significant spin–orbit coupling is usually required for the nonmagnetic materials, which is essential for the conversion of charge current to spin current. There are two major mechanisms for the conversion of charge to spin current, namely spin Hall effect^{17,18,19,20,21,22,23,24,25} and Edelstein effect.^{26} The major difference between these two effects is that spin Hall effect is usually considered as a bulk effect, which means that the spins diffuse in the direction perpendicular to the charge current, whereas the Edelstein effect is often referred as an interface effect that the spins and electrons are confined in the twodimensional (2D) state. The spin Hall effect in conventional metals and semiconductors has already been described in several review articles.^{27,28}
In this review article, we focus on the spin and charge conversion in recent quantum materials, including spinmomentum locked Rashba interfaces and topological insulator surface states, 2D materials, quasiparticles in superconductors, as well as noncollinear antiferromagnets (Fig. 2). Due to their unique spindependent properties, these quantum materials have exhibited interesting spin and charge conversion phenomena, such as giant spin and charge conversion efficiency, and gate tunable spin and charge conversion, etc. This article reviews those most important findings of quantum materials for spin and charge conversion, and is organized in the following order. The first section discusses the spin and charge conversion of Rashba states via Edelstein and inverse Edelstein effects at nonmagnetic metal interfaces, insulating oxide interfaces, and metalinsulating oxide heterostructures. The second section discusses the spinmomentum locked surface states of Bi_{2}Se_{3}type topological insulators and new types of topological insulators, including αSn and topological Kondo insulator SmB_{6}. The third section discusses the spin and charge conversion in 2D materials, including graphenebased heterostructures with large spin orbit coupling induced via proximity effect, and transition metal dichalcogenides (TMDCs), such as MoS_{2} and WTe_{2}. The fourth section discusses the quasiparticlemediated spin Hall effect in swave superconducting NbN thin films. The fifth section discusses the large anomalous Hall effect and spin Hall effect in noncollinear antiferromagnets. The final section discusses the perspectives of quantum materials for future spintronics applications.
Spin and charge conversion in Rashba interfaces
The spin and charge conversion in Rashba interfaces is often referred as Edelstein effect or RashbaEdelstein effect; a nonzero spin accumulation is accompanied with a charge current flowing in 2D asymmetric systems.^{26} At the interface, the coupling between the momentum and spin polarization directions can be expressed by the following Hamiltonian:^{26,29}
where \(\alpha _R\) is the Rashba coefficient that is proportional to the spin–orbit coupling (\(\lambda _{{\rm SO}}\)) and the electrical field (E) perpendicular to the interface (\(\alpha _R = e\lambda _{{\rm SO}}E\), e is the electron charge), \({\hat{\boldsymbol z}}\) is the unit vector perpendicular to the interface, \({\hat{\mathbf k}}\) is the wave vector, \(\hat \sigma\) is the spin Pauli matrices vector. As a result of interaction between spins and the momentum directions of the carriers, the energy dispersion exhibits two contours at the Fermi surface, as illustrated in Fig. 3a. These energy dispersion curves can be experimentally revealed by angleresolved photoemission spectroscopy (ARPES). The splitting in energy dispersion curves for spinup and spindown carriers could be used to extract the Rashba coefficient at the interface/surface, i.e., large Rashba coefficient has been identified at the interface of Bi with other metallic materials.^{30,31}
The spin and charge conversion can be explained based on the shift of the Fermi contours in the presence of electric fields. For the two Fermi contours (Fig. 3a), the inner one has spinmomentum locking feature with a clockwise spin texture, while the outer one has a counterclockwise spin texture. These two Fermi contours are symmetric without an electric field. However, in the presence of an electric field, as illustrated in Fig. 3b, both of these Fermi circles shift towards positive k_{x} direction. Shift of the outer Fermi circle gives rise to an increase in spinup density. While shift in inner Fermi circle causes an increase in spindown density. Usually, the net effect is a spinup density accompanying the charge current, since the outer Fermi circle plays the major role. Quantitatively, the generated spin density (\({\hat{\mathrm S}}\)) is proportional to charge current density (\({\hat{\mathbf J}}_{\mathbf{C}}\)), described by the following relationship:
Thus, for the efficient chargetospin conversion, a large Rashba coefficient is favored. Similar to the inverse spin Hall effect, the inverse Edelstein effect refers to that spin accumulation in inversion 2D asymmetric systems could generate an inplane electric field perpendicular to the spin polarization direction for both systems with weak and strong spin–orbit couplings.^{32,33} As illustrated in Fig. 3c, the injection of spinup polarized carriers results in the shift of the outer/inner Fermi circles to the positive/negative k_{x} direction, generating a net charge current along the positive k_{x} direction. In the last several years, intensive investigations of the Edelstein effect and inverse Edelstein effect have been performed on the Rashbasplit states at the nonmagnetic metal interfaces,^{33,34,35,36} insulating oxide interfaces,^{37,38,39,40,41} and metalinsulating oxide interfaces.^{42,43}
We first discuss the Edelstein effect and inverse Edelstein effect of the Rashba split interfaces between two metallic layers. To probe the Edelstein effect at the Ag/Bi interface, Zhang et al.^{34} have used the spinpolarized positron beam to detect the spin polarization of the outermost surface electrons in the presence of a charge current. This method is ultrasensitive to the surface spin polarization since the bound state of a positron and an electron is a Positronium. Since Positronium can only be formed for low electron density, only the outermost surface in a metal could satisfy this condition, which makes this technique ultrasensitive to the surface. During the measurement, as illustrated in Fig. 3d, a transversely spinpolarized positron beam is generated by a ^{22}Na source and an electrostatic beam apparatus, and then guided to inject into the Ag/Bi samples. A highpurity Ge detector is used to detect the Positronium annihilation γ rays, from which the component of the surface spin polarization can be obtained in the presence of a charge current flowing in the Rashba interfaces of Ag/Bi. Due to the large difference of the resistivity between Bi and Ag, the charge current mainly flows in the Ag layers. By systematically varying the thickness of Bi in the bilayer structures of αAl_{2}O_{3} (0001)/Ag (25 nm)/Bi, the chargetospin conversion effect of the Rahsba interface is investigated. For pure Ag thin films, the surface spin polarization is estimated to be 0.5% with J_{ C } = 15 A/m, which is small and most likely arising from the small spin Hall effect of Ag. A giant enhancement of the surface spin polarization is probed when the Bi thickness is ~0.3 nm with a value of 4.1% with J_{ C } = 15 A/m, which is more than ten times higher than that of pure Ag films, indicating the dominant role of the Ag/Bi interface. Figure 3e shows the Bi thickness dependence of surface spin polarization for the αAl_{2}O_{3} (0001)/Ag (25 nm)/Bi bilayer samples. Clearly, there is a strong enhancement when the Bi reaches 0.3 nm, which is approximately monolayer considering the Bi atomic radius of 0.15 nm. As the Bi thickness further increases, the detected surface spin polarization decreases, which is expected since the interface is the source for the spin generation. When the surface is far away from the interface, there is a spin depolarization due to spin scattering, following an exponential relationship (\(\exp (  d{\mathrm{/}}\lambda _{sd})\)), where λ_{ sd } is the spin diffusion length of Bi. Based on the exponential relationship (solid line in Fig. 3e), the spin diffusion length of Bi is estimated to be ~2.1 nm. Since the sign of the Rashba coefficient depends on the stacking order of Bi and Ag, reversing the Bi and Ag layer is expected to give rise to a negative surface spin polarization. Consistent with this expectation, experimental results exhibit a negative sign for the αAl_{2}O_{3} (0001)/Bi (8 nm)/Ag (25, 100, 200, 300, 400, 500 nm) bilayer samples. A large surface spin polarization of ~5% is probed when the Ag thickness is 25 nm with J_{ C } = 15 A/m. As the Ag layer thickness increases, the surface spin polarization decreases exponentially due to the spin relaxation in Ag. Since the spin–orbit coupling in Ag is much weaker than that of Bi, a much longer diffusion length of ~357 nm is observed for the surface spin polarization of the αAl_{2}O_{3} (0001)/Bi (8 nm)/Ag bilayer samples. The opposite spin polarization and its dependence on the thicknesses of Bi and Ag layers have demonstrated the dominant role of the Rashba interfaces between Bi and Ag in chargetospin conversion results.
The inverse Edelstein effect, spintocharge conversion, of Ag/Bi Rashba interface states has been investigated by the RojasSanchez et al.^{33} To generate the spin current in the Rashba interfaces, a thin NiFe (Py) layer is grown on the Bi/Ag, which acts as a spin pumping source. The spins are generated from the Py layer under its magnetization resonance conditions, which results in the generation of spin currents at the interface. This dynamic spin injection method is called spin pumping, which is a wellestablished technique to inject spin polarized carriers into various materials, including metals, semiconductors, Rashba interface states, etc.^{23,25,33,44,45} It can be considered as a process of transferring angular momentum from the FM layer into the adjacent NM layer, and the angular momentum in the NM layer is mediated by pure spin current. Figure 3f shows the schematic of the measurement setup for probing the inverse Edelstein effect in the Bi/Ag bilayer samples. At the resonance magnetic fields for the Py magnetization under certain radio frequencies, a DC pure spin current is injected into Ag and arrives at the Bi/Ag Rashba interface states; one type of spin polarized carriers move towards the Py, and the opposite type of spin polarized carriers move away from the Py. At the Bi/Ag Rashba interface states, the pure spin current is converted into a charge current in the sample’s plane (I_{ C }) due to the inverse Edelstein effect, which is probed by a voltage meter. The Bi/Ag samples are grown on a Si/SiO_{2} wafer substrate (~500 nm thermally oxidized SiO_{2}) by successive evaporation of Bi, Ag, and NiFe in ultrahigh vacuum. The texture of the Bi layer is along the crystal’s (111) direction in the rhombohedral notation, which is favored for the spintocharge conversion since relatively large Rashba coefficients have been observed by ARPES at the interface for (111)oriented Bi thin films and their heterostructures.^{30,31} Figure 3g shows the ferromagnetic resonance (FMR) spectra and measured charge currents as a function of the external magnetic field for three typical samples: 10 nm Ag/15 nm Py (left), 8 nm Bi/15 nm Py (middle) and 8 nm Bi/5 nm Ag/15 nm Py (right). For the similar FMR absorption signal, the measured charge currents of these three samples exhibit large variations. For pure Ag, the measured charge current is negligible (left), consistent with the small spin Hall angle in Ag films. For Bi films with a relatively larger spin Hall angle compared to Ag, a larger charge current is observed (middle). The largest value of the charge current is obtained on the 8 nm Bi/5 nm Ag/15 nm Py sample. Given the fact that injected spin current densities are similar for all the samples indicated by similar enhanced Gilbert damping of Py layer, the observation of largest charge current on the Bi/Ag Rashba interface strongly supports the significant spintocharge conversion arising from the large Rashba coefficient of the Bi/Ag Rasbha interface states. Besides the Bi/Ag interface, the spin and charge conversion of other Rashba interfaces, including Sb/Ag and Bi/Cu, has also been investigated via either spin pumping method or spin absorption method in a Cubased nonlocal spin valve.^{35,36}
Since the pioneering work that reported the high mobility conducting twodimensional electron gas (2DEG) between two insulating oxides (SrTiO_{3} and LaAlO_{3}),^{46} many interesting physical properties have been discovered.^{47,48} A particular interesting point is that all these physical properties are gatetunable via a perpendicular electric field. This oxide interface becomes conducting when the LaAlO_{3} layer exceeds a critical thickness of 3–4 unit cells. As illustrated in Fig. 4a, b, the polar oxide LaAlO_{3} consists of two layers, (LaO)^{+}, and (AlO_{2})^{−}, and the top surface of SrTiO_{3}, a thin TiO_{2} layer, becomes conducting. To account for the high mobility 2DEG at the interface, several mechanisms have been proposed, including the “polar catastrophe”, an electric field with thickness of the polar LaAlO_{3} layer resulting in charge transfer from the LaAlO_{3} surface to the interface,^{49} cation intermixing giving La doping in the SrTiO_{3} surface,^{50} and oxygen offstoichiometry to form SrTiO_{3x} conducting layer.^{51} Particularly intriguing for spintronics, a large Rashba coefficient has been reported via weak antilocalization measurements at T = 1.5 K^{52} and it can be markedly modulated from 1 × 10^{−12} to 5 × 10^{−12} eVm by applying an electric field. Recently, the inverse Edelstein effect of the oxide interface has been achieved experimentally and its spin and charge conversion efficiency is highly gate tunable.^{37,38}
Song et al.^{38} performed the room temperature inverse Edelstein effect experiments on the SrTiO_{3} and LaAlO_{3} interface using a thin Py metallic layer (~20 nm) as the spin pumping source. The spins are injected via spin pumping into the oxide interface, and are converted to a charge current that could be measured using a voltage meter. The angular momentum is transferred from Py to the 2DEG across the LaAlO_{3} layer via spin tunneling across the LaAlO_{3} layer and/or localized states in the LaAlO_{3} layer (i.e. oxygen vacancies). To achieve the gate tunable inverse Edelstein effect, a sample of the critical thick LaAlO_{3} layer of 3unit cell is used, of which the interfacial conductivity can be modulated dramatically by an electric field at room temperature. During the spin pumping measurement, an electrode of silver paste is used on the other side of SrTiO_{3} substrate to serve as a back gate, as schematically shown in the inset of Fig. 4c. The gate tunable spin signal of the Rashba 2DEG between SrTiO_{3} and 3unit cell LaAlO_{3} has been observed (Fig. 4c). It is clearly seen that the inverse Edelstein effect voltage (V_{IEE}), resulting from spintocharge conversion at the Rashbasplit 2DEG, can be tuned markedly by the gate voltage. Under negative gate voltages, the V_{IEE} is significantly lower, which means a lower effective spintocharge conversion, whereas, the large spin signal and low resistance of the 2DEG under positive gate voltage indicate a larger spintocharge conversion. This observation is attributed to the gate tunability of the carrier density, Rashba coefficient at the interface, and the spin pumping efficiency that is related to the spin mixing conductance between Py and the Rashba 2DEG. Furthermore, the gate dependence of the spintocharge conversion has been theoretically investigated,^{39} which shows a good agreement with the experiential results at room temperature.
Since the dielectric constant of SrTiO_{3} increases significantly at low temperature, the gate voltage modulation of the V_{IEE} at low temperatures is expected to be significantly enhanced. Indeed, at low temperature (T = 7 K), Lesne et al.^{37} reported a large gate tunable inverse Edelstein effect for the Rahsbasplit 2DEG between SrTiO_{3} and 2unit cell LaAlO_{3}, where the spintocharge conversion sign could be even reversed. The 2unit cell LaAlO_{3} is able to produce a conducting Rashba 2DEG because the critical thickness of LaAlO_{3} for the formation of the conducting 2DEG is reduced due to the deposition of ferromagnetic metallic layers, including both Co and Py.^{37,53} A large spintocharge conversion efficiency (λ_{IEE} = \(J_C^{2D}{\mathrm{/}}J_S^{3D}\)) of 6.4 nm is reported, which is more than one order larger than that of Rashba interface states between metallic layers.^{33} The gate dependence of the spintocharge conversion efficiency is shown in Fig. 4d, which clearly demonstrates the dramatic modulation of the spintocharge conversion via the perpendicular electric field. λ_{IEE} first exhibits little variation at negative gate voltages, and then changes the sign when the gate voltage is positive. The maximum value for λ_{IEE} is observed at the gate voltage of +125 V. This nontrivial gate dependence is attributed to the multiband property of the electronic structure for the Rashba 2DEG at the oxide interface. As the gate voltage modulates the carrier densities, the Fermi level shifts from a single band with d_{xy} character to other d bands, such as d_{xy} and d_{yz}. This experimental observation is supported by first principle theoretical studies that calculate a weak Rashba coefficient with a negative sign for the d_{xy} band, and a much larger Rashba coefficient for the d_{xy} and d_{yz} bands with positive sign. The carrier density across Lifshitz points corresponds to ~1.8× 10^{13} cm^{−2}, as indicated by the schematic of the band structure for the oxide interface (inset of Fig. 4d). To further confirm the scenario above, the detailed band structures are essential, which can be revealed by spinARPES measurements.
For potential applications such as magnetic switching via spin–orbit torque, the Edelstein effect, chargetospin conversion, has to be demonstrated. Recently, a significantly large spin–orbit torque arising from the Edelstein effect at the SrTiO_{3} and LaAlO_{3} interface on an adjacent CoFeB layer is reported at room temperature.^{41} Beyond the spin and charge conversion, the oxidebased interface and materials can also serve as a channel for the conducting spins, and the spin injection has been successfully performed.^{54,55,56}
Besides the Rashba states for metalmetal and oxides interfaces, the interfaces between metal and oxide have also been investigated for spin and charge conversion.^{42} Figure 4e shows the measurement geometry and the sample structure, where Py layer is the ferromagnetic layer for spin pumping source, and the Cu/Bi_{2}O_{3} is the Rashba interface that converts spin current into inplane charge current via inverse Edelstein effect. As shown in Fig. 4f, a clear spin pumping voltage owing to the spintocharge current conversion is observed around the resonance magnetic field (red curve), whereas, no spin pumping voltages could be observed on the control samples of Py/Cu (black curve) and Py/Bi_{2}O_{3} bilayers. This is understandable because Bi_{2}O_{3} is an insulator and Cu does not contribute to the conversion due to its low spin orbit coupling and weak spin Hall effect. Hence, the observed spin signal on Py/Cu/Bi_{2}O_{3} sample can only be explained by the inverse Edelstein effect of the Rashba interfacial states. A spintocharge conversion efficiency (λ_{IEE}) of ~0.6 nm is obtained, about twice the value of Bi/Ag Rashba interface.^{33} Then the interfacial Rashba coefficient is determined to be  (0.46 ± 0.06) eV Å, which might be controlled by an electric field effect similar to gate tunable inverse Edelstein effect observed at the oxide interface.^{37,38} This Rashba interface can also lead to a new type of magnetoresistance, namely Edelstein magnetoresistance,^{43} which has similar origins as spin Hall magnetoresistance observed at the interface between FM and NM with large spin Hall effect.^{57,58} This experimental work also reports that about only two thirds of the total spin relaxation occurs at the interface,^{43} which points an interesting direction for future work towards the 100% contribution from pure interface states.
Spin and charge conversion in topological insulators
Topological insulators, a class of quantum materials, have protected conducting surface or edge states, possibly arising from strong spinorbit coupling and timereversal symmetry.^{59,60} The 2D topological insulators are quantum spin Hall insulators with the transport of spin and charge only in gapless edge states. Similar to 2D topological insulators, threedimensional (3D) topological insulators have insulating bulk states and conducting surface states with spin polarization direction perpendicular to the momentum direction. This feature of the surface states is called spinmomentum locking, and has been first demonstrated by scanning tunneling microscopy and spinARPES.^{61,62} Ferromagnetic tunneling contacts have also been used to detect the spin current generation due to the spinmomentum locking property of the topological surface states.^{63,64,65,66,67} Since the spindependent chemical potentials are different between spinup and spindown carriers, the spindependent voltage measured between the ferromagnetic electrodes and the surface states is dependent on whether the magnetization is parallel or antiparallel to the spin polarization direction.^{68}
In the context of spintronics, this spinmomentum locking property could be very useful for the magnetization switching via spin–orbit torque.^{69,70,71,72} Since the spin and the momentum directions are strongly coupled to each other in the surface states of 3D topological insulators,^{73,74,75} a spin and charge conversion efficiency of 100% could be realized in ideal case. Figure 5a shows the schematic of the energy dispersion of the topological surface states. For both electron and hole carriers, the spin polarization directions are perpendicular to the momentum directions but with opposite spin textures. The spin texture direction is the property of a material that depends on the sign of surface/interfacial Rashba parameters.^{76} For Bi_{2}Se_{3}based topological insulators, the electron band has a clockwise spin texture, which results in a spindown polarization coupled to a positive momentum direction, as illustrated in Fig. 5b. While the hole band has a counterclockwise spin texture, which results in a spinup polarization coupled to a positive momentum direction, as illustrated in Fig. 5c. Due to the presence of a charge current, the Fermi circle shifts, giving rise to the accumulation of spinpolarized carriers, which is similar to the Edelstein effect of Rashba interfaces. For ntype carriers (electrons), on applying an electric field along negative k_{x} direction, the Fermi circle shifts to the positive k_{x} direction (from dashed to solid circles) and spindown electrons are accumulated at the Fermi surface, as shown in Fig. 5b. For ptype carriers (holes), on applying an electric field along negative k_{x} direction, the Fermi circle shifts to the positive k_{x} direction (from dashed to solid circles) and spinup electrons are accumulated at the Fermi surface, as shown in Fig. 5b. The spin accumulation at the surface of topological insulator (\(\left\langle {\delta S_0} \right\rangle\)) can be expressed by^{72}
where \(k_{\rm F}\) is the Fermi wavenumber, \(\delta k_x\)is the shift of Fermi circle, μ is the mobility of the topological surface states, \(E_x\) is the applied electrical field, and \(v_{\rm F}\) is the Fermi velocity. Due to the opposite sign of charge for electrons and holes, the spin and charge conversion efficiency is expected to have the same sign.
The Edelstein effect of the topological insulator surface states has been investigated using spintorque ferromagnetic resonance (STFMR) technique.^{69,71,72} The main idea of the STFMR technique is based on the ratio of spin–orbit torque due to the spin current and the Oersted field torque arising from the flow of the charge current, hence, the chargetospin conversion efficiency (q_{ICS} = \(J_S^{3D}{\mathrm{/}}J_C^{2D}\)) could be obtained. A pioneering work, done by Mellnik et al.,^{69} has demonstrated a giant chargetospin conversion efficiency in the Bi_{2}Se_{3}/Py bilayer structure at room temperature, which is much larger than the value observed in heavy metallic systems, including Pt, βTa, βW, and Bidoped Cu. Consequently, the Fermi level dependence of the topological insulators (Bi_{1−x}Sb_{ x })_{2}Te_{3} is studied to investigate the contributions from carriers in the surface states and bulk states.^{72} Figure 5d illustrates the STFMR measurement of the spin current generated from the topological insulators in the (Bi_{1−x}Sb_{ x })_{2}Te_{3} (8 nm)/Cu (8 nm)/Py (10 nm) trilayer structure, where the Cu spacing layer provides protection of the topological surface states from degradation during the deposition of the Py directly onto it. The generated spin current, carrying angular momentum, flows into the Py layer, and exerts a spin–transfer torque on the magnetization of Py controlled by an external magnetic field with an angle (θ) from the flow of the charge current (I_{C}). Figure 5e shows the Fermi level dependence of q_{ICS} for (Bi_{1−x}Sb_{ x })_{2}Te_{3}, where the position of the Fermi level is controlled by the doping ratio of Sb over Bi.^{77} In the bulk insulating (Bi_{1−x}Sb_{ x })_{2}Te_{3} samples (x from 0.5 to 0.7) at low temperature (T = 10 K), the chargetospin conversion effect via the Dirac surface states is almost constant, which is consistent with the theoretical expectation that the q_{ICS} is inversely proportional to the Fermi velocity. For the bulk conducting (Bi_{1−x}Sb_{ x })_{2}Te_{3} samples (x = 0 or 1), the estimated values of q_{ICS}, using the same analytical method, are found to be roughly equal to, or larger than those for the bulk insulating films, which might be overestimated. When the Fermi level approaches the Dirac point, q_{ICS} is remarkably reduced, which might be related to the inhomogeneity of Fermi wavenumber and/or instability of the helical spin structure. The conversion from spin current to charge current, inverse Edelstein effect, of the Bi_{2}Se_{3}based topological insulators has been studied via spin pumping from either ferromagnetic metallic layer or ferromagnetic insulators.^{78,79,80,81,82,83}
Beyond Bi_{2}Se_{3}based topological insulators, recent theoretical and experimental studies have identified new topological insulators, such as αSn and strongly correlated Kondo insulator SmB_{6}. For αSn thin films, theoretical calculations show that αSn thin films could be topological insulators via strain or quantumsize effects.^{84,85} Consequently, the helical spin polarization of the Diracconelike surface states of (001)oriented single crystalline αSn thin films, grown on InSb(001) substrates by molecular beam epitaxy, has been observed by ARPES measurements (Fig. 6a), which demonstrated that (001)oriented αSn thin film is a new 3D topological insulator.^{86} To study the spin and charge conversion in αSn topological insulator, RojasSánchez et al.^{87} performed spin pumping experiments on the (001) αSn/Ag/Fe sample, where the Ag layer (2 nm) is used to protect the topological surface states of αSn from the damage caused by growing Fe directly onto it. Figure 6b shows the FMR spectrum of the Fe and converted charge current measured on (001) αSn (30 monolayers)/Ag (2 nm)/Fe (3 nm)/Au (2 nm) sample. The spintocharge conversion efficiency is estimated to be ~2.1 nm, which is significantly larger than Rashba interfaces, such as Ag/Bi.^{33}
SmB_{6}, a Kondo insulator, has been theoretically proposed to be a topological insulator at low temperature due to the band inversion between 4f and 5d orbitals.^{88,89} Since then, several experimental studies have demonstrated that SmB_{6} is a new type of topological insulator, including spinAPERS technique, Hall transport methods, quantum oscillation measurements, etc.^{90,91,92,93,94,95} A unique property of SmB_{6} is that below ~3 K, the bulk states are insulating, and only surface carriers contribute to the conduction, as illustrated in Fig. 6c, which can be evident by the surface Hall measurement and saturation of the resistance of bulk SmB_{6} single crystals (Fig. 6d). Hence, SmB_{6} provides a platform for the clear demonstration of the Edelstein/inverse Edelstein effects for the spinmomentum locked surface states, which is quite challenging for Bi_{2}Se_{3}based topological insulators due to the presence of unavoidable bulk carriers. Song et al.^{96} observed the spintocharge conversion of the pure surface states in SmB_{6} where the spin current is generated via the spin pumping from Py, as illustrated in Fig. 6d inset. The temperature dependence of the spin pumping and inverse Edelstein effect is performed to investigate how the spin voltage evolves as the surface states emerge and become dominant. As shown in Fig. 6e, the spin voltage steadily decreases as the temperature increases, and when the temperature reaches 10 K, no obvious voltage could be detected. This observation is expected since pure surface states exist below ~3 K, giving rise to an inplane electrical voltage that is perpendicular to the spin directions, due to the inverse Edelstein effect. While more bulk carriers are activated as the temperature increases, the spin voltage is greatly suppressed due to the current shunting effect of the bulk SmB_{6} crystal. Compared to Bi_{2}Se_{3}based topological insulators, both αSn and Kondo insulator SmB_{6} have counterclockwise helical spin configuration of the electrontype Fermi contours, resulting in the opposite sign of spintocharge conversion signal.^{76,86,87,93,96}
Up to date, a large range of the spin and charge efficiency values from ~0.001 to ~2 has been reported for the topological insulators, using different techniques including STFMR, spin pumping and inverse Edelstein effect, magnetization switching, and second harmonic measurement, etc.^{66,69,70,71,72,78,79,80,81,82,83,87,97,98} Even for the same measurement on the same topological insulator, i.e., second harmonic measurement of the spin–orbit torque arising from 3D topological insulators, different values have been reported.^{70,99} One possible reason is related to the multiple sources of second harmonic voltages, i.e., large unidirectional magnetoresistance is also reported at the topological insulator/FM interface.^{100}
To fully address the disagreement of the exact value for spin and charge conversion efficiency generated from the surface states of 3D topological insulators, future experimental and theoretical studies are essential. Despite this disagreement, it has been demonstrated that 3D topological insulators can be used to perform efficient magnetization switching for FM films with both inplane and perpendicular magnetic anisotropies at room temperature.^{97,98}
Spin and charge conversion in 2D materials
The isolation of graphene and related 2D materials has created new opportunities for spintronics. For example, graphene is potentially useful for spin channels in spin transistor and logic devices due to long spin lifetime and spin diffusion length.^{8,9,73,101} TMDCs are potentially useful for spintronics and valleytronics devices arising from the spinvalley coupling.^{102,103} Regarding the spin current generation/detection, it has been recently demonstrated that 2D materials can be potentially used for efficient spin and charge conversion, including graphene with large spin orbit coupling due to proximity effect with other materials, TMDCs with low crystalline symmetry (MoS_{2} and WTe_{2}).
Although the intrinsic spin orbit coupling is rather weak in pristine graphene, it can be largely enhanced via proximity effect with other materials that have large spin orbit coupling, such as ferromagnetic insulator, Yttrium Iron Garnet (YIG),^{104,105,106} and TMDCs,^{107,108} etc. Recently, it has been shown that YIG/graphene could be a promising material candidate for efficient spin and charge conversion.^{105,106} The spin current is generated via spin pumping from YIG thin film grown on GGG substrates (Fig. 7a), and then converted to a charge current in graphene due to the enhanced spin–orbit coupling and inverse Edelstein effect. The spin signal arising from the charge current flowing in graphene is measured via two Ag contacts at the ends of graphene channel. The typical magnetic field dependence curves of the spin pumping voltage measured on YIG/Graphene are shown in Fig. 7b. When the external magnetic field is applied along the graphene channel (ϕ = 90°), the pumped spin polarized carriers will be converted to a charge current perpendicular to the graphene channel. Thus, no spin pumping voltage could be detected (black line in Fig. 7b). When the external magnetic field is applied perpendicular to the graphene channel (ϕ = 0° and 180°), the pumped spin polarized carriers will be converted to a charge current with a direction along the graphene channel, giving rise to spin pumping voltages (red and blue lines in Fig. 7b). Furthermore, ionic liquid gating provides a large electric field on the graphene surface, which has been demonstrated to strongly modulate the spintocharge conversion efficiency of YIG/graphene.^{106}
Different from pristine graphene, TMDCs are usually with large spin–orbit coupling arising from the large intrinsic spin–orbit coupling of the heavy elements, such as Mo and W.^{102} As a result, the spin splitting at the surface due to broken inversion symmetry could be used for converting spin current to/from charge current and switching the magnetization of nanomagnets. Both STFMR technique and spin pumping method have been used to study the spin and charge conversion in monolayer MoS_{2}.^{109,110} The STFMR results on monolayer MoS_{2}/Py exhibit a large spin–orbit torque generated by the Edelstein effect of thin MoS_{2} films. Specifically, a very large dampinglike torque, relative to a fieldlike torque, has been identified.^{109} The spin pumping results on monolayer MoS_{2}/Al (3 nm)/Co (10 nm) present a large spintocharge conversion efficiency that corresponds to an effective spin Hall angle of ~12. Besides, the spintocharge conversion efficiency could be manipulated via a back gate voltage across a 300 nm insulating SiO_{2} layer.^{110}
Very interestingly, recent experimental results show a large outofplane spin–orbit torque in WTe_{2} arising from the low crystalline symmetry.^{111} The surface crystalline structure of WTe_{2} belongs to the space group \({\mathrm{Pmn2}}_{\mathrm{1}}\), and the crystal structure near the surface is shown in Fig. 7c. For the WTe_{2}/Py bilayer samples, a mirror symmetry exists with respect to the bc plane (dashed red line), but does not exist with respect to ac plane, which means that there is no 180° rotational symmetry about the caxis (perpendicular to the sample plane). As a result, an outofplane spin–orbit torque is allowed by symmetry for the current flowing along the aaxis of a WTe_{2}/Py bilayer. Specifically, a charge current flowing along positive aaxis gives rise to an extra spin–orbit torque that is along negative caxis, while a charge current flowing along negative aaxis gives rise to an extra spin–orbit torque that is along positive caxis. As the inplane magneticfield angle (ϕ) changes with current applied parallel to the aaxis, the symmetric voltage arising from inplane spin–orbit torque has a twofold rotational symmetry, which changes sign when the magnetization is rotated inplane by 180°. This is expected since the inplane spin–orbit torque is proportional to the angle between magnetization and inplane spin polarization due to the charge current via spin Hall effect and/or Edelstein effect. However, the magnetic field angle dependence of the asymmetric voltage due to outofplane spin–orbit torque does not have a twofold rotational symmetry, thus cannot be well fitted by the cos(ϕ)sin(2ϕ) relationship expected for pure Oersted field torque, as shown in Fig. 7d. This result indicates the existence of another outofplane spin–orbit torque besides the Oersted field torque. This extra outofplane torque changes sign when the charge current switches direction, and is allowed for WTe_{2}/Py bilayer devices which also do not have twofold symmetry when the current is along aaxis. If the charge current flows along baxis of WTe_{2}/Py bilayer devices, a twofold symmetry of the asymmetry voltage is observed. These results demonstrate the possibility of generating efficient spin–orbit torque based on the TMDCs and other materials with broken crystal symmetry and significant spin–orbit coupling.
Quasiparticlemediated spin Hall effect in superconductors
Superconductor spintronics is an emerging field focusing on the interplay between superconductivity and spintronics.^{112} In the FM/superconductor heterostructures, the magnetization of FM layer can strongly modulate the superconducting critical temperature of the superconducting layer.^{113,114,115,116} Spin dynamics of superconducting films could be measured via spin pumping from an adjacent ferromagnetic insulating layer, which has been recently theoretically proposed and experimentally investigated.^{117,118} The underlying mechanism is that the magnetization dynamics, probed by FMR and spin pumping, is coupled to the spin dynamics of the superconductor via the interfacial s–d exchange interaction. In the content of spintronics, the spin polarization of a FM material can be probed using superconducting point contact via the differential conductance measurement since the Andreev reflection at the interface is determined by the spin polarized density of states.^{119} Recently, many extraordinary spindependent physical properties of superconductors have been observed. For instance, large magnetoresistance has been achieved in the spin valve consisting of a superconducting layer between two ferromagnetic films.^{115} This large magnetoresistance is attributed to the different superconducting temperatures for the parallel and antiparallel states of the two FM layers’ magnetization. Besides, extremely long spin lifetimes and large spin Hall effect have been discovered for superconductors mediated by quasiparticles, the superpositions of electronlike and holelike excitations. The values of the spin lifetime and spin Hall effect exceed several orders compared to those of the normal states above the superconducting temperature.^{120,121,122} Here, we discuss experimental results of the quasiparticlesmediated large spin Hall effect in swave superconducting NbN thin films.
Quasiparticlemediated spin Hall effect of a swave superconductor is first theoretically studied, which predicts a large enhancement below the superconducting critical temperature.^{120,123} Experimentally, Wakamura et al.^{122} have demonstrated the large spin Hall effect of quasiparticles in NbN thin films, using the spin absorption technique based on a Cu nonlocal spin valve.^{24,124} As illustrated in Fig. 8a, the spin current is injected from Py electrode (spin injector), and then diffuses inside the Cu spin channel. The spin polarization direction is controlled via the external magnetic field, which sets the magnetization direction of the Py electrode (spin injector). When the spin current arrives at the Cu/NbN interface, spins are absorbed by the NbN with significant spin–orbit coupling. Different from Cu, where spins are carried by electrons, the spins in NbN are carried by quasiparticles, and converted to a quasiparticlemediated charge imbalance (J_{Q}) due to the inverse spin Hall effect. The spin absorption at the Cu/NbN interface can be viewed as the angular momentum transfer between the spins of electrons in the Cu and the spins of quasiparticles in superconducting NbN. The inverse spin Hall signal has been investigated across the superconducting critical temperature of NbN. Above the superconducting temperature (T = 20 K and higher), a regular inverse spin Hall effect is observed and the spin Hall angle is estimated to be ~0.9%. The spin Hall angle exhibits tiny difference between 20 K and 300 K (~0.9–1.3%) and no dependence on the charge current is observed. However, below the superconducting critical temperature, a large inverse spin Hall signal is observed at T = 3 K, which is more than 2000 times larger compared to the inverse spin Hall signal at 20 K. Figure 8b compares the current dependences of the inverse spin Hall signal between T = 3 K and 20 K, where the inverse spin Hall resistance is normalized by the value at 20 K (ΔR_{ISHE}^{normal}) under the spin injection current of 300 µA. The strong spin current dependence of inverse spin Hall signal for quasiparticles is attributed to the increase of the local temperature at the Cu/NbN interface due to the Joule heating. Hence, when a large spin injection current is applied, the real temperature around the Cu/NbN interface increases, which results in the large suppression of the superconducting gap of NbN at the interface.
A critical parameter for the quasiparticlemediated spin Hall effect is the length scale (λ_{Q}) as illustrated in Fig. 8c. After the formation of the quasiparticlemediated charge current via inverse spin Hall effect, the quasiparticles will condensate into Coopers pairs, which gives rise to a charge imbalance effect and a spacingdependent inverse spin Hall voltage signal. When the voltage probes are far away from the Cu/NbN interface (d2 in Fig. 8c), the charge imbalance or inverse spin Hall signal is not observable. Figure 8d compares the inverse spin Hall signal for two devices with different distances (d1 = 400 nm and d2 = 10 µm) from the Cu/NbN interfaces measured at T = 3 K with a spin injection current of 1 µA. A tiny inverse spin Hall signal for the device with d2 = 10 µm is observed, which is markedly suppressed compared to the device with d1 = 400 nm.
Both the spin injection current and the voltage probe distance dependences of the inverse spin Hall signal confirm that the inverse spin Hall effect is mediated by the quasiparticles of the superconducting NbN layer. This novel mechanism mediated by quasiparticles gives rise to a huge enhancement of the inverse spin Hall effect, which is more than 2000 times larger than that in the normal state mediated by electrons in the presence of spin–orbit coupling. These results pave the way to realize a sensitive spin detector with superconductors. To use superconductors as spin generators, quasiparticlemediated spin Hall effect which generates spin current from quasiparticle charge imbalance needs future studies.
Anomalous Hall and spin Hall effects in noncollinear antiferromagnets
Since the early work done by Edwin Hall on ferromagnetic metals,^{125} anomalous Hall effect has been intensively studied, from the mechanisms (intrinsic, skew scattering, side jump scattering) to various materials including ferromagnetic metals, diluted ferromagnetic semiconductors, and heavy fermions, etc.^{126,127,128} Different from the anomalous Hall effect in FM, which is usually assumed to be proportional to its magnetization, the noncollinear antiferromagnets are predicted to hold a large anomalous Hall effect arising from a realspace Berry phase effect despite almost zero net magnetization.^{128,129,130,131,132,133,134} Chen et al.^{133} performed the calculation on IrMn_{3}, of which Mn sublattices consist of 2D kagome lattices viewed from its (111) direction. They theoretically demonstrate that a large anomalous Hall effect exists, arising from the mirror symmetry breaking and spin–orbit coupling. The total magnetization is calculated to be ∼0.02 μ_{B} per formula unit along the (111) direction and the intrinsic anomalous Hall conductivity is 218 Ω^{−1} cm^{−1}.
Shortly after the theoretical studies, two experimental groups have observed the large anomalous Hall effect in noncollinear antiferromagnets.^{135,136} Nakatsuji et al.^{135} found a large anomalous Hall effect in Mn_{3}Sn, an antiferromagnet that has a 120degree spin order at room temperature. As shown in Fig. 9a, each ab plane consists of a slightly distorted kagome lattice of Mn moments each of ~3 μ_{B}, and a very small net ferromagnetic moment of ~0.002 μ_{B} per Mn atom arises from the geometrical frustration. Since only one of the three Mn moments is parallel to the local easyaxis towards its nearestneighboring Sn sites, the canting of the other two spins towards the local easyaxis is considered to result in the weak net ferromagnetic moment, which allows the switching of the sign of net magnetization and the anomalous Hall effect via an external magnetic field. By subtracting the ordinary Hall effect, anomalous Hall effect due to magnetization, the anomalous Hall effect due to the noncollinear spin order (\(\rho _H^{AF}\)) could be obtained, which can be described by the following equation:
where \(\rho _H\) is the total Hall resistivity, R_{0} is the ordinary Hall coefficient, B is the external magnetic field, R_{ s } is the regular anomalous Hall coefficient that is related to magnetization, μ_{0} is the permeability, and M is the magnetization. The external magnetic field dependence of \(\rho _H^{AF}\)at T = 300 K is shown in Fig. 9b, from which a strong facet dependence is observed. When the current is along the crystal’s [0001] direction, and the magnetic field is along [01\(\bar 1\)0] direction, the largest anomalous Hall effect is observed, whereas, no anomalous Hall effect is observed when the current is along the crystal’s [01\(\bar 1\)0] direction, and the magnetic field is along [0001] direction. This facet dependence is consistent with the magnetic field dependence of the magnetization arising from the staggered moments of the noncollinear spin structure. The switching of the magnetization also corresponds to changing the spinchirality of the noncollinear antiferromagnetic order, which gives rise to the sign switching of \(\rho _H^{AF}\). Besides Mn_{3}Sn, a large anomalous Hall effect has also been observed on Heusler compound Mn_{3}Ge,^{136} which has the similar crystalline structure as Mn_{3}Sn. A much larger anomalous Hall conductivity is observed in Mn_{3}Ge, which is nearly three times higher than that of Mn_{3}Sn. Recently, the anomalous Nernst effect and magnetooptical Kerr effect of Mn_{3}Sn has also been investigated.^{137,138,139} A large transverse Seebeck coefficient ~0.35–0.6 µV K^{−1} at zero magnetic field is observed from 200 to 300 K. A large zerofield Kerr rotation angle of 20 mdeg is observed at room temperature, comparable to ferromagnetic metals.^{139} Also, a large topological Hall effect has been reported in Mn_{5}Si_{3}, when the spin arrangement changes from collinear to noncollinear as the temperature decreases, suggesting the origin of the topological Hall effect is the noncollinear magnetic structure.^{140}
The spin Hall effect, the conversion between charge and spin currents, shares the same origin as the anomalous Hall effect: relativistic spin–orbit coupling generates an asymmetric deflection of the charge carriers depending on their spin direction.^{28,128} Both recent experimental and theoretical studies have demonstrated the considerably large spin Hall effect due to the noncollinear spin order.^{141,142} As shown in Fig. 9c, the spinup and spindown carriers flow in the opposite directions, resulting in the generation of a spin current. Zhang et al.^{141} studied the chargetospin conversion in single crystalline IrMn_{3} films by measuring the spin–orbit torque on a thin Py layer at room temperature using the STFMR technique. IrMn_{3} is known to display a triangular chiral magnetic structure with the Mn magnetic moments aligned at 120° to each other in the (111) plane when the Ir and Mn atoms are chemically ordered. In the cubic IrMn_{3} lattice the Mn atoms are arranged in the form of triangles within the (111) plane of the primitive unit cell. A large spin Hall angle is observed in (001) oriented single crystalline antiferromagnetic IrMn_{3} thin films, which is ~2 times larger than that of the (111) oriented IrMn_{3} films. The strong facet dependence of the effective spin Hall angle of IrMn_{3} (Fig. 9d) identifies two distinct mechanisms for generation of spin current from charge carriers; the first mechanism, which is facetindependent, arises from conventional bulk spindependent scattering within the IrMn_{3} layer. And the second intrinsic mechanism derives from the noncollinear antiferromagnetic structure. The effective spin Hall effect of the second mechanism can be dramatically enhanced by manipulating the populations of the various antiferromagnetic domains, i.e., a ~75% enhancement of the effective spin Hall angle is achieved by perpendicular magnetic field annealing on the 3 nm (001) IrMn_{3} thin film. The reconfiguration of the antiferromagnetic domain structure of the IrMn_{3} layer can be reconfigured due to exchange coupling with the Py layer when it is cooled from a temperature above its blocking temperature to room temperature. Further experimental evidences also support the novel mechanism of the spin Hall effect due to the noncollinear spin order. The insertion of a thin Au layer is used to weaken the exchange coupling between Py and IrMn_{3}, resulting in the largely reduced dependence of the effective spin Hall angle on the crystalline orientations. Besides, the facet dependence of the effective spin Hall angle disappears for CuAuItype antiferromagnets (Ir_{1x}Mn_{ x } with x ~53 and 64%) with collinear spin order.
One of the possible origins of these interesting spindependent properties is associated to significant enhancement of the Berry curvature, particularly around band crossing points called Weyl points near the Fermi energy.^{135,137,141,142,143} Direct experimental evidences of the Mn_{3}Sn and Mn_{3}Ge as Weyl semimetals, such as surface Fermi Arcs via spinAPRES, have not been reported yet.^{143} The proposal using the spin–orbit torque and antiferromagnetic order to control the topological properties of Weyl semimetals is quite intriguing.^{144}
Summary and outlook
In conclusion, the conversion between spin and charge using quantum materials has attracted a great deal of attention recently and quantum materials have exhibited unique spindependent properties. Looking forward, novel mechanisms that can generate spin current would be particularly interesting, arising from crystalline symmetry, or coupling with other degrees of freedom, such as phonon, magnon, spinon, and valley/layer degree of freedom, etc.^{103,145,146,147,148} The spin and charge conversion in these quantum materials could be also very important for the detection of the spin current generated via various mechanisms,^{146} the probe of the nontrivial magnetic fluctuations,^{149,150,151,152} and search for new quantum states.^{153,154} Besides, the efficient spin current generation may pave the way for future spintronics device applications, including magnetic random accessory memory, domain wall Racetrack memory, and skyrmion Racetrack memory, etc.^{155,156,157,158}
References
Maekawa, S., Valenzuela, S. O., Saitoh, E. & Kimura, T. Spin Current. (Oxford University Press, Oxford, UK, 2012).
Wolf, S. A. et al. Spintronics: a spinbased electronics vision for the future. Science 294, 1488–1495 (2001).
Zutic, I., Fabian, J. & Das Sarma, S. Spintronics: fundamentals and applications. Rev. Mod. Phys. 76, 323–410 (2004).
Datta, S. & Das, B. Electronic analog of the electrooptic modulator. Appl. Phys. Lett. 56, 665–667 (1990).
Dery, H., Dalal, P., Cywinski, L. & Sham, L. J. Spinbased logic in semiconductors for reconfigurable largescale circuits. Nature 447, 573–576 (2007).
BehinAein, B., Datta, D., Salahuddin, S. & Datta, S. Proposal for an allspin logic device with builtin memory. Nat. Nanotechnol. 5, 266–270 (2010).
Koo, H. C. et al. Control of spin precession in a spininjected field effect transistor. Science 325, 1515–1518 (2009).
Han, W., Kawakami, R. K., Gmitra, M. & Fabian, J. Graphene spintronics. Nat. Nanotech. 9, 794–807 (2014).
Roche, S. et al. Graphene spintronics: the European Flagship perspective. 2D Mater. 2, 030202 (2015).
Ralph, D. C. & Stiles, M. D. Spin transfer torques. J. Magn. Magn. Mater. 320, 1190–1216 (2008).
Brataas, A., Kent, A. D. & Ohno, H. Currentinduced torques in magnetic materials. Nat. Mater. 11, 372–381 (2012).
Miron, I. M. et al. Perpendicular switching of a single ferromagnetic layer induced by inplane current injection. Nature 476, 189–193 (2011).
Liu, L. et al. Spintorque switching with the giant spin Hall effect of tantalum. Science 336, 555–558 (2012).
Brataas, A. & Hals, K. M. D. Spin–orbit torques in action. Nat. Nanotech. 9, 86–88 (2014).
Yu, G. et al. Switching of perpendicular magnetization by spin–orbit torques in the absence of external magnetic fields. Nat. Nanotech. 9, 548–554 (2014).
Fukami, S., Anekawa, T., Zhang, C. & Ohno, H. A spin–orbit torque switching scheme with collinear magnetic easy axis and current configuration. Nat. Nanotech. 11, 621–625 (2016).
Dyakonov, M. I. & Perel, V. I. Spin relaxation of conduction electrons in noncentrosymmetric semiconductors. Sov. Phys. Solid State 13, 3023–3026 (1972).
Zhang, S. Spin Hall effect in the presence of spin diffusion. Phys. Rev. Lett. 85, 393–396 (2000).
Hirsch, J. E. Spin Hall effect. Phys. Rev. Lett. 83, 1834–1837 (1999).
Kato, Y., Myers, R., Gossard, A. & Awschalom, D. Observation of the spin Hall effect in semiconductors. Science 306, 1910–1913 (2004).
Sinova, J. et al. Universal intrinsic spinHall effect. Phys. Rev. Lett. 92, 126603 (2004).
Valenzuela, S. O. & Tinkham, M. Direct electronic measurement of the spin Hall effect. Nature 442, 176–179 (2006).
Saitoh, E., Ueda, M., Miyajima, H. & Tatara, G. Conversion of spin current into charge current at room temperature: inverse spinHall effect. Appl. Phys. Lett. 88, 182509 (2006).
Kimura, T., Otani, Y., Sato, T., Takahashi, S. & Maekawa, S. Room temperature reversible spin Hall effect. Phys. Rev. Lett. 98, 156601 (2007).
Mosendz, O. et al. Quantifying spin Hall Angles from spin pumping: experiments and theory. Phys. Rev. Lett. 104, 046601 (2010).
Edelstein, V. M. Spin polarization of conduction electrons induced by electric current in twodimensional asymmetric electron systems. Solid State Commun. 73, 233–235 (1990).
Jungwirth, T., Wunderlich, J. & Olejnik, K. Spin Hall effect devices. Nat. Mater. 11, 382–390 (2012).
Sinova, J., Valenzuela, S. O., Wunderlich, J., Back, C. H. & Jungwirth, T. Spin Hall effects. Rev. Mod. Phys. 87, 1213–1260 (2015).
Manchon, A., Koo, H. C., Nitta, J., Frolov, S. M. & Duine, R. A. New perspectives for Rashba spin–orbit coupling. Nat. Mater. 14, 871–882 (2015).
Koroteev, Y. M. et al. Strong spin–orbit splitting on Bi surfaces. Phys. Rev. Lett. 93, 046403 (2004).
Ast, C. R. et al. Giant spin splitting through surface alloying. Phys. Rev. Lett. 98, 186807 (2007).
Shen, K., Vignale, G. & Raimondi, R. Microscopic theory of the inverse Edelstein effect. Phys. Rev. Lett. 112, 096601 (2014).
Sánchez, J. C. R. et al. Spintocharge conversion using Rashba coupling at the interface between nonmagnetic materials. Nat. Commun. 4, 3944 (2013).
Zhang, H. J. et al. Chargetospin conversion and spin diffusion in Bi/Ag bilayers observed by spinpolarized positron beam. Phys. Rev. Lett. 114, 166602 (2015).
Zhang, W., Jungfleisch, M. B., Jiang, W., Pearson, J. E. & Hoffmann, A. Spin pumping and inverse RashbaEdelstein effect in NiFe/Ag/Bi and NiFe/Ag/Sb. J. Appl. Phys. 117, 17C727 (2015).
Isasa, M. et al. Origin of inverse RashbaEdelstein effect detected at the Cu/Bi interface using lateral spin valves. Phys. Rev. B 93, 014420 (2016).
Lesne, E. et al. Highly efficient and tunable spintocharge conversion through Rashba coupling at oxide interfaces. Nat. Mater. 15, 1261–1266 (2016).
Song, Q. et al. Observation of inverse Edelstein effect in Rashbasplit 2DEG between SrTiO_{3} and LaAlO_{3} at room temperature. Sci. Adv. 3, e1602312 (2017).
Seibold, G., Caprara, S., Grilli, M. & Raimondi, R. Theory of the spin galvanic effect at oxide interfaces. Phys. Rev. Lett. 119, 256801 (2017).
Chauleau, J. Y. et al. Efficient spintocharge conversion in the 2D electron liquid at the LAO/STO interface. Europhys. Lett. 116, 17006 (2016).
Wang, Y. et al. Roomtemperature giant chargetospin conversion at the SrTiO_{3}–LaAlO_{3} oxide interface. Nano Lett. 17, 7659–7664 (2017).
Karube, S., Kondou, K. & Otani, Y. Experimental observation of spintocharge current conversion at nonmagnetic metal/Bi_{2}O_{3} interfaces. Appl. Phys. Expr. 9, 033001 (2016).
Kim, J. et al. Evaluation of bulkinterface contributions to Edelstein magnetoresistance at metal/oxide interfaces. Phys. Rev. B 96, 140409 (2017).
Tserkovnyak, Y., Brataas, A., Bauer, G. E. W. & Halperin, B. I. Nonlocal magnetization dynamics in ferromagnetic heterostructures. Rev. Mod. Phys. 77, 1375–1421 (2005).
Ando, K. et al. Electrically tunable spin injector free from the impedance mismatch problem. Nat. Mater. 10, 655–659 (2011).
Ohtomo, A. & Hwang, H. Y. A highmobility electron gas at the LaAlO3/SrTiO3 heterointerface. Nature 427, 423–426 (2004).
Hwang, H. Y. et al. Emergent phenomena at oxide interfaces. Nat. Mater. 11, 103–113 (2012).
Mannhart, J. & Schlom, D. G. Oxide interfaces—an opportunity for electronics. Science 327, 1607–1611 (2010).
Okamoto, S., & Millis, A. J. Electronic reconstruction at an interface between a Mott insulator and a band insulator. Nature 428, 630–633 (2004)..
Chambers, S. A. Understanding the mechanism of conductivity at the LaAlO3/SrTiO3(001) interface. Surf. Sci. 605, 1133–1140 (2011).
Herranz, G. et al. High Mobility in LaAlO_{3}/SrTiO_{3} heterostructures: origin, dimensionality, and perspectives. Phys. Rev. Lett. 98, 216803 (2007).
Caviglia, A. D. et al. Tunable Rashba spin–orbit interaction at oxide interfaces. Phys. Rev. Lett. 104, 126803 (2010).
Lesne, E. et al. Suppression of the critical thickness threshold for conductivity at the LaAlO_{3}/SrTiO_{3} interface. Nat. Commun. 5, 4291 (2014).
Reyren, N. et al. Gatecontrolled spin injection at LaAlO_{3}/SrTiO_{3} interfaces. Phys. Rev. Lett. 108, 186802 (2012).
Han, W. et al. Spin injection and detection in lanthanum and niobiumdoped SrTiO3 using the Hanle technique. Nat. Commun. 4, 2134 (2013).
Ohshima, R. et al. Realization of delectron spin transport at room temperature at a LaAlO_{3}/SrTiO_{3} interface. Nat. Mater. 16, 609–614 (2017).
Nakayama, H. et al. Spin Hall Magnetoresistance Induced by a nonequilibrium proximity effect. Phys. Rev. Lett. 110, 206601 (2013).
Chen, Y.T. et al. Theory of spin Hall magnetoresistance. Phys. Rev. B 87, 144411 (2013).
Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators. Rev. Mod. Phys. 82, 3045–3067 (2010).
Qi, X.L. & Zhang, S.C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057–1110 (2011).
Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime. Nature 460, 1101–1105 (2009).
Roushan, P. et al. Topological surface states protected from backscattering by chiral spin texture. Nature 460, 1106–1109 (2009).
Li, C. H. et al. Electrical detection of chargecurrentinduced spin polarization due to spinmomentum locking in Bi_{2}Se. Nat. Nanotechnol. 9, 218–224 (2014).
Tang, J. et al. Electrical detection of spinpolarized surface states conduction in (Bi_{0.53}Sb_{0.47})_{2}Te topological insulator. Nano Lett. 14, 5423–5429 (2014).
Ando, Y. et al. Electrical detection of the spin polarization due to charge flow in the surface state of the topological insulator Bi_{1.5}Sb_{0.5}Te_{1.7}Se_{1.3}. Nano Lett. 14, 6226–6230 (2014).
Liu, L. et al. Spinpolarized tunneling study of spinmomentum locking in topological insulators. Phys. Rev. B 91, 235437 (2015).
Tian, J., Hong, S., Miotkowski, I., Datta, S. & Chen, Y. P. Observation of currentinduced, longlived persistent spin polarization in a topological insulator: a rechargeable spin battery. Sci. Adv. 3, e1602531 (2017).
Hong, S., Diep, V., Datta, S. & Chen, Y. P. Modeling potentiometric measurements in topological insulators including parallel channels. Phys. Rev. B 86, 085131 (2012).
Mellnik, A. R. et al. Spin–transfer torque generated by a topological insulator. Nature 511, 449–451 (2014).
Fan, Y. et al. Magnetization switching through giant spin–orbit torque in a magnetically doped topological insulator heterostructure. Nat. Mater. 13, 699–704 (2014).
Wang, Y. et al. Topological surface states originated spin–orbit torques in Bi2Se3. Phys. Rev. Lett. 114, 257202 (2015).
Kondou, K. et al. Fermileveldependent chargetospin current conversion by Dirac surface states of topological insulators. Nat. Phys. 12, 1027–1031 (2016).
Pesin, D. & MacDonald, A. H. Spintronics and pseudospintronics in graphene and topological insulators. Nat. Mater. 11, 409–416 (2012).
Yazyev, O. V., Moore, J. E. & Louie, S. G. Spin polarization and transport of surface states in the topological insulators Bi2Se3 and Bi2Te3 from first principles. Phys. Rev. Lett. 105, 266806 (2010).
Zhang, S. & Fert, A. Conversion between spin and charge currents with topological insulators. Phys. Rev. B 94, 184423 (2016).
Yu, R., Weng, H., Fang, Z. & Dai, X. Pseudospin, realspin and spin polarization of photoemitted electrons. Phys. Rev. B 94, 085123 (2016).
Zhang, J. et al. Band structure engineering in (Bi_{1−x}Sb_{x})_{2}Te_{3} ternary topological insulators. Nat. Commun. 2, 574 (2011).
Shiomi, Y. et al. Spinelectricity conversion induced by spin injection into topological insulators. Phys. Rev. Lett. 113, 196601 (2014).
Deorani, P. et al. Observation of inverse spin Hall effect in bismuth selenide. Phys. Rev. B 90, 094403 (2014).
Yamamoto, K. T., Shiomi, Y., Segawa, K., Ando, Y. & Saitoh, E. Universal scaling for the spinelectricity conversion on surface states of topological insulators. Phys. Rev. B 94, 024404 (2016).
Jamali, M. et al. Giant spin pumping and inverse spin Hall effect in the presence of surface and bulk spin–orbit coupling of topological insulator Bi_{2}Se_{3}. Nano Lett. 15, 7126–7132 (2015).
Mendes, J. B. S. et al. Diracsurfacestatedominated spin to charge current conversion in the topological insulator (Bi_{0.22}Sb_{0.78})_{2}Te_{3} films at room temperature. Phys. Rev. B 96, 180415 (2017).
Wang, H. et al. Surfacestatedominated spin–charge current conversion in topologicalinsulator/ferromagneticinsulator heterostructures. Phys. Rev. Lett. 117, 076601 (2016).
Xu, Y. et al. Largegap quantum spin Hall insulators in tin films. Phys. Rev. Lett. 111, 136804 (2013).
Barfuss, A. et al. Elemental topological insulator with tunable fermi level: strained αSn on InSb(001). Phys. Rev. Lett. 111, 157205 (2013).
Ohtsubo, Y., Le Fèvre, P., Bertran, F. & TalebIbrahimi, A. Dirac cone with helical spin polarization in ultrathin αSn(001) Films. Phys. Rev. Lett. 111, 216401 (2013).
RojasSánchez, J. C. et al. Spin to charge conversion at room temperature by spin pumping into a new type of topological insulator: αSn films. Phys. Rev. Lett. 116, 096602 (2016).
Dzero, M., Sun, K., Galitski, V. & Coleman, P. Topological Kondo insulators. Phys. Rev. Lett. 104, 106408 (2010).
Lu, F., Zhao, J., Weng, H., Fang, Z. & Dai, X. Correlated topological insulators with mixed valence. Phys. Rev. Lett. 110, 096401 (2013).
Kim, D. J., Xia, J. & Fisk, Z. Topological surface state in the Kondo insulator samarium hexaboride. Nat. Mater. 13, 466–470 (2014).
Li, G. et al. Twodimensional fermi surfaces in Kondo insulator SmB_{6}. Science 346, 1208–1212 (2014).
Jiang, J. et al. Observation of possible topological ingap surface states in the Kondo insulator SmB_{6} by photoemission. Nat. Commun. 4, 3010 (2013).
Xu, N. et al. Direct observation of the spin texture in SmB_{6} as evidence of the topological Kondo insulator. Nat. Commun. 5, 4566 (2014).
Syers, P., Kim, D., Fuhrer, M. S. & Paglione, J. Tuning bulk and surface conduction in the proposed topological Kondo insulator SmB6. Phys. Rev. Lett. 114, 096601 (2015).
Dzero, M., Xia, J., Galitski, V. & Coleman, P. Topological Kondo insulators. Annu. Rev. Condens. Matter Phys. 7, 249–280 (2016).
Song, Q. et al. Spin injection and inverse Edelstein effect in the surface states of topological Kondo insulator SmB_{6}. Nat. Commun. 7, 13485 (2016).
Han, J. et al. Roomtemperature spin–orbit torque switching induced by a topological insulator. Phys. Rev. Lett. 119, 077702 (2017).
Wang, Y. et al. Room temperature magnetization switching in topological insulator–ferromagnet heterostructures by spin–orbit torques. Nat. Commun. 8, 1364 (2017).
Yasuda, K. et al. Currentnonlinear Hall effect and spin–orbit torque magnetization switching in a magnetic topological insulator. Phys. Rev. Lett. 119, 137204 (2017).
Yasuda, K. et al. Large unidirectional magnetoresistance in a magnetic topological insulator. Phys. Rev. Lett. 117, 127202 (2016).
Han, W. Perspectives for spintronics in 2D materials. APL Mater. 4, 032401 (2016).
Xiao, D., Liu, G.B., Feng, W., Xu, X. & Yao, W. Coupled spin and valley physics in monolayers of MoS2 and other groupVI dichalcogenides. Phys. Rev. Lett. 108, 196802 (2012).
Xu, X., Yao, W., Xiao, D. & Heinz, T. F. Spin and pseudospins in layered transition metal dichalcogenides. Nat. Phys. 10, 343–350 (2014).
Wang, Z., Tang, C., Sachs, R., Barlas, Y. & Shi, J. Proximityinduced ferromagnetism in graphene revealed by the anomalous Hall effect. Phys. Rev. Lett. 114, 016603 (2015).
Mendes, J. B. S. et al. Spincurrent to chargecurrent conversion and magnetoresistance in a hybrid structure of graphene and yttrium iron garnet. Phys. Rev. Lett. 115, 226601 (2015).
Dushenko, S. et al. Gatetunable spin–charge conversion and the role of spin–orbit interaction in graphene. Phys. Rev. Lett. 116, 166102 (2016).
Gmitra, M. & Fabian, J. Graphene on transitionmetal dichalcogenides: a platform for proximity spin–orbit physics and optospintronics. Phys. Rev. B 92, 155403 (2015).
Wang, Z. et al. Strong interfaceinduced spin–orbit interaction in graphene on WS_{2}. Nat. Commun. 6, 8339 (2015).
Zhang, W. et al. Research update: spin transfer torques in permalloy on monolayer MoS_{2}. APL Mater. 4, 032302 (2016).
Cheng, C. et al. Spin to charge conversion in MoS_{2} monolayer with spin pumping. Preprint at arXiv:1510.03451, (2016).
MacNeill, D. et al. Control of spin–orbit torques through crystal symmetry in WTe_{2}/ferromagnet bilayers. Nat. Phys. 13, 300–305 (2016).
Linder, J. & Robinson, J. W. A. Superconducting spintronics. Nat. Phys. 11, 307–315 (2015).
Gu, J. Y. et al. Magnetizationorientation dependence of the superconducting transition temperature in the ferromagnet–superconductor–ferromagnet system: CuNi/Nb/CuNi. Phys. Rev. Lett. 89, 267001 (2002).
Yang, Z., Lange, M., Volodin, A., Szymczak, R. & Moshchalkov, V. V. Domainwall superconductivity in superconductorferromagnet hybrids. Nat. Mater. 3, 793–798 (2004).
Miao, G.X., Yoon, K., Santos, T. S. & Moodera, J. S. Influence of spinpolarized current on superconductivity and the realization of large magnetoresistance. Phys. Rev. Lett. 98, 267001 (2007).
Xiao, J. Q. & Chien, C. L. Proximity effects in superconductor/insulatingferromagnet NbNm/GdN multilayers. Phys. Rev. Lett. 76, 1727–1730 (1996).
Inoue, M., Ichioka, M. & Adachi, H. Spin pumping into superconductors: a new probe of spin dynamics in a superconducting thin film. Phys. Rev. B 96, 024414 (2017).
Yao, Y. et al. Probe of spin dynamics in superconducting NbN thin films via spin pumping. Preprint at arXiv:1710.10833 (2017).
Soulen, R. J. Jr et al. Measuring the spin polarization of a metal with a superconducting point contact. Science 282, 85–88 (1998).
Yamashita, T., Takahashi, S., Imamura, H. & Maekawa, S. Spin transport and relaxation in superconductors. Phys. Rev. B 65, 172509 (2002).
Yang, H., Yang, S.H., Takahashi, S., Maekawa, S. & Parkin, S. S. P. Extremely long quasiparticle spin lifetimes in superconducting aluminium using MgO tunnel spin injectors. Nat. Mater. 9, 586–593 (2010).
Wakamura, T. et al. Quasiparticlemediated spin Hall effect in a superconductor. Nat. Mater. 14, 675–678 (2015).
Kontani, H., Goryo, J. & Hirashima, D. S. Intrinsic spin Hall effect in the $s$wave superconducting state: analysis of the Rashba model. Phys. Rev. Lett. 102, 086602 (2009).
Niimi, Y. et al. Giant spin Hall effect induced by skew scattering from bismuth impurities inside thin film CuBi alloys. Phys. Rev. Lett. 109, 156602 (2012).
Hall, E. H. XXXVIII. On the new action of magnetism on a permanent electric current. Philos. Mag. 10, 301–328 (1880).
Sundaram, G. & Niu, Q. Wavepacket dynamics in slowly perturbed crystals: gradient corrections and Berryphase effects. Phys. Rev. B 59, 14915–14925 (1999).
Tian, Y., Ye, L. & Jin, X. Proper scaling of the anomalous Hall effect. Phys. Rev. Lett. 103, 087206 (2009).
Nagaosa, N., Sinova, J., Onoda, S., MacDonald, A. H. & Ong, N. P. Anomalous Hall effect. Rev. Mod. Phys. 82, 1539 (2010).
Yamanaka, M., Koshibae, W. & Maekawa, S. “Flux” state in the doubleexchange model. Phys. Rev. Lett. 81, 5604–5607 (1998).
Ye, J. et al. Berry phase theory of the anomalous Hall effect: application to colossal magnetoresistance manganites. Phys. Rev. Lett. 83, 3737–3740 (1999).
Ohgushi, K., Murakami, S. & Nagaosa, N. Spin anisotropy and quantum Hall effect in the kagom/‘e lattice: chiral spin state based on a ferromagnet. Phys. Rev. B 62, R6065–R6068 (2000).
Shindou, R. & Nagaosa, N. Orbital ferromagnetism and anomalous Hall effect in antiferromagnets on the distorted fcc lattice. Phys. Rev. Lett. 87, 116801 (2001).
Chen, H., Niu, Q. & MacDonald, A. H. Anomalous Hall effect arising from noncollinear antiferromagnetism. Phys. Rev. Lett. 112, 017205 (2014).
Kübler, J. & Felser, C. Noncollinear antiferromagnets and the anomalous Hall effect. Europhys. Lett. 108, 67001 (2014).
Nakatsuji, S., Kiyohara, N. & Higo, T. Large anomalous Hall effect in a noncollinear antiferromagnet at room temperature. Nature 527, 212–215 (2015).
Nayak, A. K. et al. Large anomalous Hall effect driven by a nonvanishing Berry curvature in the noncolinear antiferromagnet Mn_{3}Ge. Sci. Adv. 2, e1501870 (2016).
Ikhlas, M. et al. Large anomalous Nernst effect at room temperature in a chiral antiferromagnet. Nat. Phys. 13, 1085 (2017).
Li, X. et al. Anomalous Nernst and RighiLeduc effects in Mn_{3}Sn: Berry curvature and entropy flow. Phys. Rev. Lett. 119, 056601 (2017).
Higo, T. et al. Large magnetooptical Kerr effect and imaging of magnetic octupole domains in an antiferromagnetic metal. Nat. Photon. 12, 73–78 (2018).
Sürgers, C., Fischer, G., Winkel, P. & Löhneysen, H. V. Large topological Hall effect in the noncollinear phase of an antiferromagnet. Nat. Commun. 5, 3400 (2014).
Zhang, W. et al. Giant facetdependent spinorbit torque and spin Hall conductivity in the triangular antiferromagnet IrMn_{3}. Sci. Adv. 2, e1600759 (2016).
Železný, J., Zhang, Y., Felser, C. & Yan, B. Spinpolarized current in noncollinear antiferromagnets. Phys. Rev. Lett. 119, 187204 (2017).
Hao, Y. et al. Topological Weyl semimetals in the chiral antiferromagnetic materials Mn_{3}Ge and Mn_{3}Sn. New J. Phys. 19, 015008 (2017).
Šmejkal, L., Železný, J., Sinova, J. & Jungwirth, T. Electric control of Dirac quasiparticles by spin–orbit torque in an antiferromagnet. Phys. Rev. Lett. 118, 106402 (2017).
Uchida, K. et al. Observation of the spin Seebeck effect. Nature 455, 778–781 (2008).
Otani, Y., Shiraishi, M., Oiwa, A., Saitoh, E. & Murakami, S. Spin conversion on the nanoscale. Nat. Phys. 13, 829 (2017).
Bauer, G. E. W., Saitoh, E. & van Wees, B. J. Spin caloritronics. Nat. Mater. 11, 391–399 (2012).
Matsuo, M., Ieda, J. I., Harii, K., Saitoh, E. & Maekawa, S. Mechanical generation of spin current by spin–rotation coupling. Phys. Rev. B 87, 180402 (2013).
Niimi, Y. et al. Strong suppression of the spin Hall effect in the spin glass state. Phys. Rev. Lett. 115, 196602 (2015).
Qiu, Z. et al. Spincurrent probe for phase transition in an insulator. Nat. Commun. 7, 12670 (2016).
Wang, H., Du, C., Hammel, P. C. & Yang, F. Spin transport in antiferromagnetic insulators mediated by magnetic correlations. Phys. Rev. B 91, 220410 (2015).
Lin, W., Chen, K., Zhang, S. & Chien, C. L. Enhancement of thermally injected spin current through an antiferromagnetic insulator. Phys. Rev. Lett. 116, 186601 (2016).
Hirobe, D. et al. Onedimensional spinon spin currents. Nat. Phys. 13, 30–34 (2016).
Yuan, W. et al. Experimental signatures of spin superfluid ground state in canted antiferromagnet Cr_{2}O_{3} via nonlocal spin transport. Sci. Adv. 4, eaat1098 (2018).
Parkin, S. S. P. et al. Magnetically engineered spintronic sensors and memory. Proc. IEEE 91, 661–680 (2003).
Parkin, S. S. P., Hyayshi, M. & Thomas, L. Magnetic domainwall racetrack memory. Science 320, 190–194 (2008).
Parkin, S. & Yang, S.H. Memory on the racetrack. Nat. Nanotech. 10, 195–198 (2015).
Fert, A., Cros, V. & Sampaio, J. Skyrmions on the track. Nat. Nanotech. 8, 152–156 (2013).
Acknowledgements
We are grateful to Wenyu Xing and Yunyan Yao for their help preparing illustrations. W.H. acknowledges the financial support from National Basic Research Programs of China (Grant nos. 2015CB921104 and 2014CB920902), National Natural Science Foundation of China (No. 11574006) and the 1000 Talents Program for Young Scientists of China. Y.O. acknowledges the financial support from GrantinAid for Scientific Research on Innovative Area, “Nano Spin Conversion Science” (Grant no. 26103002) and CREST (Grant no. JPMJCR15Q5). S.M. acknowledges the financial support from ERATOJST (JPMJER1402), and KAKENHI (No. 26103006 and No. JP17H02927) from MEXT, Japan.
Author information
Authors and Affiliations
Contributions
The manuscript was written through contributions of all authors. W.H. wrote the paper and Y.O. and S.M. examined and improved it.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Han, W., Otani, Y. & Maekawa, S. Quantum materials for spin and charge conversion. npj Quant Mater 3, 27 (2018). https://doi.org/10.1038/s4153501801009
Received:
Revised:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4153501801009
This article is cited by

Interfacial magnetic spin Hall effect in van der Waals Fe3GeTe2/MoTe2 heterostructure
Nature Communications (2024)

Magnetodynamic properties of ultrathin films of Fe\(_{\textbf{3}}\)Sn\(_{\textbf{2}}\)a topological kagome ferromagnet
Scientific Reports (2024)

Phase transitions associated with magneticfield induced topological orbital momenta in a noncollinear antiferromagnet
Nature Communications (2024)

Achieving environmental stability in an atomically thin quantum spin Hall insulator via graphene intercalation
Nature Communications (2024)

Reversal of spinpolarization near the Fermi level of the Rashba semiconductor BiTeCl
npj Quantum Materials (2023)